Structural Variability versus Structural Flexibility. A Case Study of Eu9Cd4+xSb9 and Ca9Mn4+xSb9 (x ≈ (1)/2).
Liu, Xiao-Cun; Wu, Zhen; Xia, Sheng-Qing; Tao, Xu-Tang; Bobev, Svilen; Inorganic chemistry 54 (2015) 947–955; doi:10.1021/ic5023505

data_4341705
_publ_section_title
;
 Structural Variability versus Structural Flexibility. A Case Study of
 Eu9Cd4+xSb9 and Ca9Mn4+xSb9 (x &#x2248; (1)/2).
;
_journal_issue                   3
_journal_name_full               'Inorganic chemistry'
_journal_page_first              947
_journal_page_last               955
_journal_paper_doi               10.1021/ic5023505
_journal_volume                  54
_journal_year                    2015
_chemical_formula_sum            'As9 Ca9 Zn4.46'
_chemical_formula_weight         1326.39
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           62
_symmetry_cell_setting           orthorhombic
_symmetry_space_group_name_Hall  '-P 2ac 2n'
_symmetry_space_group_name_H-M   'P n m a'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   11.855(2)
_cell_length_b                   4.2747(8)
_cell_length_c                   41.440(8)
_cell_measurement_reflns_used    539
_cell_measurement_temperature    296(2)
_cell_measurement_theta_max      20.06
_cell_measurement_theta_min      5.72
_cell_volume                     2100.0(7)
_computing_cell_refinement       'Bruker SMART'
_computing_data_collection       'Bruker SMART'
_computing_data_reduction        'Bruker SAINT'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      296(2)
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 1.000
_diffrn_measurement_device_type  'Bruker APEX-II CCD'
_diffrn_measurement_method       '\f and \w scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.1899
_diffrn_reflns_av_sigmaI/netI    0.0974
_diffrn_reflns_limit_h_max       15
_diffrn_reflns_limit_h_min       -15
_diffrn_reflns_limit_k_max       5
_diffrn_reflns_limit_k_min       -5
_diffrn_reflns_limit_l_max       53
_diffrn_reflns_limit_l_min       -53
_diffrn_reflns_number            24023
_diffrn_reflns_theta_full        27.10
_diffrn_reflns_theta_max         27.10
_diffrn_reflns_theta_min         0.98
_exptl_absorpt_coefficient_mu    21.277
_exptl_absorpt_correction_T_max  0.7408
_exptl_absorpt_correction_T_min  0.5678
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   'SADABS (Sheldrick,2003)'
_exptl_crystal_colour            black
_exptl_crystal_density_diffrn    4.195
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       irregular
_exptl_crystal_F_000             2443
_exptl_crystal_size_max          0.03
_exptl_crystal_size_mid          0.03
_exptl_crystal_size_min          0.02
_refine_diff_density_max         3.466
_refine_diff_density_min         -1.486
_refine_diff_density_rms         0.349
_refine_ls_extinction_coef       0.00029(3)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc^2^\l^3^/sin(2\q)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   0.999
_refine_ls_matrix_type           full
_refine_ls_number_parameters     157
_refine_ls_number_reflns         2647
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      0.999
_refine_ls_R_factor_all          0.1118
_refine_ls_R_factor_gt           0.0494
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0280P)^2^+0.0000P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0792
_refine_ls_wR_factor_ref         0.0970
_reflns_number_gt                1559
_reflns_number_total             2647
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ic5023505_si_002.cif
_cod_data_source_block           III
_cod_depositor_comments
;
The following automatic conversions were performed:

'_symmetry_cell_setting' value 'Orthorhombic' changed to
'orthorhombic' according to
/home/saulius/struct/COD-crude-data--automatic-downloads/rss-feeds/ACS/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from 2011-04-26.

Automatic conversion script
Id: cif_fix_values 2935 2014-11-11 08:27:57Z andrius 

 Adding full bibliography for 4341703--4341709.cif.
;
_cod_original_cell_volume        2100.1(7)
_cod_original_sg_symbol_H-M      Pnma
_cod_database_code               4341705